**Optical study of Dirac fermions and related phonon anomalies in the antiferromagnetic**

**compound CaFeAsF**

B. Xu,1,2_{H. Xiao,}1,*_{B. Gao,}1_{Y. H. Ma,}3_{G. Mu,}3_{P. Marsik,}2_{E. Sheveleva,}2_{F. Lyzwa,}2_{Y. M. Dai,}4
R. P. S. M. Lobo,5,6_{and C. Bernhard}2,*†*

1_{Center for High Pressure Science and Technology Advanced Research, Beijing 100094, China}

2* _{University of Fribourg, Department of Physics and Fribourg Center for Nanomaterials, Chemin du Musée 3, CH-1700 Fribourg, Switzerland}*
3

_{State Key Laboratory of Functional Materials for Informatics and Shanghai Center for Superconductivity, Shanghai Institute of Microsystem}*and Information Technology, Chinese Academy of Sciences, Shanghai 200050, China*

4_{Center for Superconducting Physics and Materials, National Laboratory of Solid State Microstructures and Department of Physics,}

*Nanjing University, Nanjing 210093, China*

5* _{LPEM, ESPCI Paris, PSL University, CNRS, F-75231 Paris Cedex 5, France}*
6

_{Sorbonne Université, CNRS, LPEM, F-75005 Paris Cedex 5, France}(Received 16 February 2018; published 8 May 2018)

We performed optical studies on CaFeAsF single crystals, a parent compound of the 1111-type iron-based
*superconductors that undergoes a structural phase transition from tetragonal to orthorhombic at Ts*= 121 K and

*a magnetic one to a spin density wave (SDW) state at TN*= 110 K. In the low-temperature optical conductivity

spectrum, after the subtraction of a narrow Drude peak, we observe a pronounced singularity around 300 cm−1 that separates two regions of quasilinear conductivity. We outline that these characteristic absorption features are signatures of Dirac fermions, similar to what was previously reported for the BaFe2As2system [Z.-G. Chen

*et al.,***Phys. Rev. Lett. 119**,096401(2017)]. In support of this interpretation, we show that for the latter system
this singular feature disappears rapidly upon electron and hole doping, as expected if it arises from a van Hove
singularity in between two Dirac cones. Finally, we show that one of the infrared-active phonon modes (the Fe-As
mode at 250 cm−1) develops a strongly asymmetric line shape in the SDW state and note that this behavior can
be explained in terms of a strong coupling with the Dirac fermions.

DOI:10.1103/PhysRevB.97.195110

**I. INTRODUCTION**

The discovery of high-temperature superconductivity in the iron-based superconductors (IBSs) has attracted extensive attention [1,2]. IBSs are multiband materials with a Fermi surface that is composed of disconnected hole and electron sheets [3–5]. This multiband structure leads to rich physics, where interband antiferromagnetic interactions are crucial for high-temperature superconductivity [3,4]. Contrary to the Mott insulating state of the cuprates, the parent antiferromagnetic phase of the IBSs has a metallic character [6] and possesses nontrivial topological properties with Dirac fermions near the Fermi energy [7,8]. The formation of the Dirac fermion state occurs near the nodes of the spin-density-wave (SDW) gap that involves several bands and leads to complex zone folding effects [7]. The existence of a Dirac cone in BaFe2As2has been first reported from angle-resolved photoemission spectroscopy and magnetic quantum oscillation measurements [9,10]. Sub-sequent, theoretical and experimental studies revealed that the Dirac cones exist in pairs [11,12]. More recently, magneto-optical experiments have demonstrated that the Dirac fermion state in BaFe2As2and SrFe2As2is two-dimensional [13]. The observation of such a Dirac fermion state with protected Dirac

*_{hong.xiao@hpstar.ac.cn}
*†*_{christian.bernhard@unifr.ch}

cones in the IBSs’ parent compounds provides us with a new kind of topological material, after cuprates [14], graphene [15], topological insulators [16,17], and Weyl semimetals [18,19]. It likely inspires new research that might even unravel a connection between Dirac fermions and superconductivity.

CaFeAsF is a parent compound of the 1111-type family of
the IBSs. It is isostructural to LaFeAsO and exhibits a transition
*from a tetragonal to an orthorhombic phase at Ts* = 121 K that

is well separated from an antiferromagnetic transition into a
*SDW phase at TN*= 110 K [20,21]. This is different from

the parent compound of the 122 phase for which these two
transitions coincide [22]. Upon a partial substitution of Fe by
*Co, CaFeAsF becomes superconducting with a maximum Tc*of

22 K [23]. More impressively, in rare-earth doped compounds,
*Tc*as high as 56 K can be obtained [24]. However, the study on

CaFeAsF is limited due to the small size of the single crystal and its poor quality. Recently, high-quality single crystals of CaFeAsF with a size above 1 mm were successfully grown by a self-flux method [21]. The availability of such sizable single crystals allows for an optical study of the intrinsic properties of the 1111-type IBSs, such as the nodal SDW and the resulting Dirac fermion states.

The optical conductivity probes the bulk band structure and carrier electrodynamics over a broad energy range and provides rich information on the intraband and interband transitions of possible Dirac cones. Although optical investigations into the parent compounds of IBSs have been conducted by many

groups [25–33], the optical signatures of the Dirac fermions have so far been only discussed for the 122 compound [13]. The evolution of these Dirac fermions with electron and hole doping has also not yet been reported. We fill this gap by performing a systematic optical study on single crystals of the CaFeAsF parent compound which reveals clear spectro-scopic signatures of the Dirac fermions. Furthermore, for the BaFe2As2 compound, we study how these Dirac fermions evolve as a function of electron and hole doping. Finally, in CaFeAsF we observe an anomalous line shape of the Fe-As mode which provides evidence that it strongly interacts with the Dirac fermions.

**II. EXPERIMENTAL METHOD**

High-quality single crystals of CaFeAsF were grown using
the self-flux method with a CaAs flux [21]. Their electronic and
magnetic properties and the structural and antiferromagnetic
*transition temperatures of Ts* *= 121 K and TN*= 110 K,

respectively, were reported in Ref. [21]. High-quality single
crystals of BaFe2As2 and its electron- and hole-doped
com-pounds [Ba(Fe*0.985*Co*0.015*)2As2and Ba*0.92*K*0.08*Fe2As2] were
synthesized with the methods described in the cited references
[34,35]. The ab-plane reflectivity R(ω) was measured at a
near-normal angle of incidence on Bruker VERTEX 70Vand

IFS66V *FTIR spectrometers with an in situ gold overfilling*
technique [36]. Data from 50 to 12000 cm−1 were collected
at different temperatures with a ARS-Helitran crysostat. The
room temperature spectrum in the near-infrared to ultraviolet
range (4000–50000 cm−1) was obtained with a commercial
ellipsometer (Woollam VASE). The optical conductivity was
*obtained by performing a Kramers-Kronig analysis of R(ω)*
[37]. For the low-frequency extrapolation below 50 cm−1, we
*used a Hagen-Rubens function (R= 1 − A*√*ω*). For the
ex-trapolation on the high-frequency side, we assumed a constant
reflectivity up to 12.5 eV that is followed by a free-electron
*(ω*−4) response.

**III. RESULTS AND DISCUSSION**

Figure 1 *displays the spectra of the reflectivity R(ω)*
[Fig.1(a)] and the optical conductivity σ1*(ω) [Fig.* 1(b)] of
CaFeAsF up to 2000 cm−1 at several selected temperatures.
Insets (c) and (e) show the room temperature spectra over a
larger range up to 50000 cm−1. In the low-frequency region,
*R(ω) shows a typical metallic response, i.e., it approaches*
unity at low frequencies and increases upon cooling. The
corresponding conductivity spectra exhibit a Drude-like peak
centered at zero frequency. The metallic response is also
*evident from the dc resistivity in inset (d) of Fig.* 1(a) as
determined from a transport measurement (solid line) and
from the optical conductivity (open symbols). Upon entering
*the SDW state, R(ω) exhibits a clear suppression between*
200 and 1000 cm−1 and an enhancement between 1000 and
2000 cm−1*. Correspondingly, the optical conductivity σ*1*(ω)*
gets suppressed below ∼800 cm−1 in the SDW state and
the resulting missing spectral weight is transferred to higher
frequencies up to a range of about 2000 cm−1. Although
the spectral weight of the Drude-like contribution is strongly
reduced in the SDW state, it remains finite to the lowest
temperature. The same kind of characteristic spectral features

FIG. 1. (a) Far-infrared reflectivity of CaFeAsF at different
tem-peratures. Inset (c), 300-K reflectivity over a broad frequency range;
*inset (d), comparison of the dc resistivity ρab* (solid line) with the

zero-frequency values of the Drude fits to the conductivity data (open circles). (b) Far-infrared optical conductivity of CaFeAsF at different temperatures. Inset (e), optical conductivity at 300 K over a broad frequency range.

due to the formation of a SDW gap were observed in 122-type AFe2As2 (A = Ba, Sr, and Ca) single crystals [25–27], as well as in 1111-type LaFeAsO [38,39]. This suggests that these undoped parent compounds have similar electronic and magnetic properties. In particular, the persistence of a finite Drude response to low temperature signifies that the SDW gap develops only on parts of the Fermi surface.

For a quantitative analysis we fitted the optical spectra with
a Drude-Lorentz model,
*σ*1*(ω)*=
*2π*
*Z*_{0}
2
*pD*
*ω*2_{τ}*D*+* _{τD}*1
+

*k*

*γkω*2

*Sk*2

*ω*2

*22*

_{0,k}− ω*+ γ*2

*kω*2

*,*(1)

*where Z*0 is the vacuum impedance. The first term describes the free-carrier Drude response, characterized by a plasma

*frequency pD*

*and a scattering rate 1/τD*. The squared

*frequency, *2

*pD∝ n/m, is a measure of the ratio of the electron*

*density n, and their effective mass m. The second term contains*
a sum of Lorentz oscillators for which each has a resonance
*frequency ω0,k, a line width γk, and an oscillator strength Sk*.

The corresponding fit to the conductivity at 10 K (thick blue line) using the function of Eq. (1) (thick red line) is shown in the inset of Fig.2(a). As shown by the thin colored lines, the

FIG. 2. (a) Optical conductivity of CaFeAsF after subtraction of
the Drude and phonon terms in the antiferromagnetic state. The red
dashed lines through the data are linear guides to the eye. The red
*arrow indicates a possible van Hove singularity. (Inset) Fit of σ*1*(ω)*

at 10 K with the Drude-Lorentz model. (b) Temperature dependence
*of the Drude spectral weight SD(T ) and the restricted spectral weight*

*S*2000cm−1

800cm−1 *(T ). (c) Temperature dependence of the scattering rate 1/τD*

*of the Drude term. The solid line represents a T*2_{behavior. The vertical}

*dashed line denotes the structural transition temperature Ts*.

fitting curve is decomposed into one Drude term representing
the response of free carriers, two Lorentz terms depicting the
broader electronic peaks around 300 and 1000 cm−1, two
Lorentz terms for the two sharp phonons, as well as a Lorentz
term that accounts for the interband transitions at higher energy.
With this fit configuration we could also describe with equal
*quality the σ*1*(ω) curves at all temperatures.*

Figure2(b)shows the temperature dependence of the Drude
*weight, SD(T )*=*π*

2

*Z*0

2

*pD*, obtained from these fits with Eq. (1).

*Above Ts, SD(T ) is almost temperature independent and*

*reflects the weak temperature dependence of σ*1*(ω). Toward*
lower temperatures there is a strong decrease of the Drude
weight due to the opening of the SDW gap. In agreement with
a nodal nature of the SDW gap, the Drude weight is strongly
suppressed but remains finite at low temperature. Notably,
the onset of this decrease is rather sharp and occurs around
*Ts* *(marked by the dashed red line) rather than at TN*. This

result demonstrates that the electronic state near the structural
phase transition is already very close to that in the magnetic
state, which may imply an intimate relationship between the
structural and magnetic transitions [40–42]. A corresponding
effect is seen in Fig2(c)*for the scattering rate 1/τD*, which

*also shows a strong reduction that sets in below Ts*. This strong

reduction of the scattering rate can also be explained in terms
of the Dirac-cone-like band dispersion at the nodes of the SDW
gap [7,9]. The red solid line denotes a T2*fit of 1/τD*that spans

*the entire temperature range below Ts* and is suggestive of a

Fermi-liquid behavior.

Figure2(a)shows the conductivity spectra at 10 and 75 K,
after the contribution of the Drude response and the sharp
phonon modes have been subtracted to emphasize the singular
structure of the low-energy absorption peak. For the 10-K
spec-trum it clearly reveals a singular kink around 300 cm−1and two
quasilinear regions toward lower and higher frequencies shown
by the red dashed lines. The spectrum at 75 K confirms that with
*the temperature increasing toward Ts* this kink weakens and

becomes less singular. It also shows that the linearly increasing
part of the conductivity at lower and higher frequencies is
hardly temperature dependent. This confirms that the missing
spectral weight of the Drude peak is transferred to the broad
band around 1000 cm−1that corresponds to the SDW gap. This
assignment is supported by the temperature dependence of the
*restricted spectral weight, defined as S(T )*=* _{ωa}ωbσ*1

*(ω,T )dω,*

*with the cutoff frequencies ωa*= 800 cm−1

*and ωb*=

2000 cm−1, that is shown by the blue diamonds in Fig.2(b).
Next, we discuss in more detail the origin of the singular
absorption feature around 300 cm−1. In most of the previous
studies of BaFe2As2it was attributed to a second, smaller SDW
gap [25–29]. However, a real challenge for this interpretation
has been provided by the optical spectra of a detwinned
BaFe2As2 single crystal for which the absorption peak in
*the response along the b axis acquires a very singular shape*
[29]. More recently, the magnetic-field dependence of this
absorption feature has been interpreted in terms of an interband
transition of two-dimensional Dirac fermions [13] that appear
in the nodal regions of the SDW gap due to band backfolding
effects. Here, we follow up on this interpretation for which the
Dirac nodes are protected by the combination of the physical
symmetry and the topology of the band structure [7,9,10].
The linear slope of the conductivity in Fig. 2(a) is typical
for the linear band dispersion of Dirac fermions [43,44]. The
additional singular kink around 300 cm−1 is characteristic
of the single-point singularity in Weyl semimetals, where a
van Hove singularity due to saddle points of the conduction
and valance bands arises between a pair of Dirac cones with
opposite chiralities [45–47]. In the pnictides case, theory also
predicts a pair of Dirac cones but with the same chirality
[11]. These similarities between CaFeAsF and Dirac fermion
materials suggest that the observed features are related to the
contributions of Dirac fermions. Meanwhile, the presence of
the finite Drude response at low frequencies, representing the
intraband transition contributions of the Dirac cones, suggests
a nonzero chemical potential (relative to the Fermi level) of
the Dirac nodes, which would result in a redistribution of the
low-energy spectral weight between intraband and interband
transitions. In addition, we should notice that in CaFeAsF
*σ*1*(ω) is almost frequency independent in the range between*
300 and 600 cm−1if the contributions of other interband
tran-sitions at higher frequencies are subtracted. Such plateaulike
*behavior of σ*1*(ω) is indicative of the optical response of*
two-dimensional Dirac cones [13,48,49], which is similar to
what has been predicted and observed in graphene [50,51].
Very recently, the existence of Dirac fermions in CaFeAsF has
been confirmed by quantum oscillation measurements [48].

This connection between the singular features in the low-frequency part of the optical response and the Dirac nodes in

FIG. 3. (a) Optical conductivity of undoped, Co (electron)-, and K (hole)-doped BaFe2As2at 5 K. The inset shows the infrared-active

phonon and the corresponding Fano fits. (b) The subtracted spectra in the low-energy region. The diagram shows a schematic band dispersion of a pair of Dirac cones with the same chirality [11].

the parent compounds of the IBSs has been further tested by
studying how they evolve as a function of electron and hole
doping. Figure3 *shows the corresponding σ*1*(ω) spectra (at*
5 K) for the parent compound BaFe2As2(black line) as well
as for weakly electron doped Ba(Fe,Co)2As2 (red line), and
weakly hole doped (Ba,K)Fe2As2 (blue line). For both cases
the kink feature can be seen to diminish very rapidly. A very
weak feature is still visible at the same energy for the more
weakly doped Ba(Fe,Co)2As2. This can be readily understood
in terms of the sketch of the band structure in the vicinity
of a pair of Dirac cones carrying the same chirality that is
shown in Fig.3(b)and describes the expected behavior in the
antiferromagnetic state of an IBS’s parent compound [11]. The
red arrow indicates the interband transitions between the two
saddle points in the middle of the pair of Dirac cones, which
*give rise to the singular kink in σ*1*(ω). This singular feature*
*exists only as long as the chemical potential (EF*) is located

between the two saddle points. Thus it diminishes rather
*rapidly as EF* is shifted upwards (downwards) upon electron

*(hole) doping and vanishes as soon as EF*is located outside the

energy window between these two saddle points (red and blue
*dotted lines). The position of EF* with respect to these saddle

points can also change for different parent compounds such as for the family of AFe2As2with A= Ba, Sr, and Ca [25–27]. The reported optical data show indeed that this singularity is more pronounced for Ba than for Sr and essentially absent for CaFe2As2 [25–27]. The latter behavior of CaFe2As2 agrees

FIG. 4. (a) Line shape of the infrared-active phonon modes at
temperatures from 300 to 10 K. The black solid lines through
the data denote the Fano fits. (b)–(d) Temperature dependence of
*the resonance position ω*0*, intensity *2*, and Fano parameter 1/q*2

of the two phonons. The vertical dashed line denotes the structural
*transition temperature Ts*.

*with a theoretical calculation which predicts that EF*is located

outside the energy window of the saddle points [11].

Next, we turn to the anomalous temperature dependence
of the line shape of the phonon modes across the
antifer-romagnetic transition in CaFeAsF. As shown in Fig. 1, in
addition to the gross features, two sharp peaks representing
*the symmetry allowed in-plane infrared active Eu* phonon

modes are observed around 250 and 265 cm−1. The mode
at lower frequency (phonon A) is assigned to the in-plane
displacement of the Fe-As ions, which is similar to the phonon
features observed at the same energy in 122-type AFe2As2
[25–28] and 1111-type ReFeAsO (Re= La, Nd, and Sm) [39].
The other mode (phonon B), which is located at significantly
higher frequency in ReFeAsO [39], is associated with the
in-plane displacement of the F-Ca ions. Figure4(a)shows an
*enlarged view of σ*1*(ω) in the relevant frequency region of*
235–285 cm−1, where the two phonon modes are seen more
clearly and several interesting features can be identified. First,
*the position of phonon A shifts discontinuously at Ts*, while

phonon B does not show a corresponding renormalization across the structural and magnetic transitions. Secondly, the line shapes for both phonon modes become rather asymmetric toward low temperatures. Such an asymmetric line shape is characteristic of a strong coupling between the phonons and some electronic excitations.

The asymmetry of the phonon has been quantified by fitting with a so-called Fano model [52] that can be written as

*σ*1*(ω)*=
*2π*
*Z*0
2
*γ*
*q*2_{+}*4q(ω−ω*0)
*γ* − 1
*q*2_{1}+*4(ω−ω*0)2
*γ*2
* ,* (2)

*where ω*0*, γ , and represent the resonance frequency, line*
width, and strength of the phonon, respectively. The asymmetry
of this Fano-type line shape is described by the dimensionless
*parameter 1/q*2* _{. As 1/q}*2

_{increases, the line shape becomes}more asymmetric, indicating a larger coupling strength. In

*the case of 1/q*2 _{= 0, a symmetric Lorentz-type line shape}
is recovered.

Figure 4(a) shows the corresponding fits of the phonon
line shapes at different temperatures (black solid lines) which
describe the measured spectra rather well. Figures4(b)–4(d)
show the temperature dependence of the fitting parameters
*ω*0*, *2*, and 1/q*2. Clearly, phonon A is much more strongly
renormalized across the structural and magnetic transitions
than phonon B. It exhibits pronounced anomalies in all three
fitting parameters similar to the case of BaFe2As2 [28,30].
*Nevertheless, the low-temperature value of 1/q*2 * _{ 0.1 of}*
phonon A is much larger than the one for BaFe2As2

*(1/q*2

*0.016) [30]. This corresponds to a much larger asymmetry*of the phonon line shape and thus a larger coupling strength between the phonon and the electronic excitations in CaFeAsF. The much weaker normalization of the phonon B suggests that the lattice vibrations associated with the F-Ca ions are less sensitive to the structural and magnetic transitions and the related changes of the electronic structure.

It should be noted that the Dirac fermions may be responsi-ble for the enhanced electron-phonon coupling in CaFeAsF. In Dirac materials, the Dirac nodes are located in close proximity to the Fermi level, and the corresponding excitations occur at very low energy. When this energy scale overlaps with the phonon resonance, a strong coupling between the Dirac fermions and phonon can arise and manifest itself in a strong Fano resonance [53–55]. Indeed, in CaFeAsF the low-energy absorption associated with the Dirac fermions, especially the enhanced singular absorption around 300 cm−1, is rather close the phonon resonance at 255 cm−1. The weaker electron phonon coupling in BaFe2As2thus can be explained in terms of a small blue shift of the singular absorption feature which occurs, here, around 350 cm−1. Furthermore, the inset of Fig.3(a)shows the evolution of the asymmetry of the phonon mode in Ba(Fe,Co)2As2 and (Ba,K)Fe2As2, which confirms that its strength is correlated with the one of the singular absorption feature.

Finally, we discuss the possible anisotropic optical re-sponses of the Dirac fermions in the parent compounds. A recent theoretical study has revealed that the optical response of the Fermi arc surface states of a Dirac semimetal can be strongly anisotropic with respect to the polarization direction of the light, i.e., whether it is polarized along or transverse

to the Fermi arc [56]. This may also explain the pronounced
anisotropy of the optical response that has been observed in
po-larized infrared studies of detwinned BaFe2As2crystals [29].
There the singularity in the electronic part and the anomaly
of the Fe-As phonon mode become much more pronounced
*along the b-axis direction than along the a-axis direction. In*
analogy, this can be understood in terms of an anisotropic
light-matter interaction which depends on whether the light
polarization is parallel or perpendicular to the line connecting
the pair of Dirac nodes. This calls for further polarized infrared
studies on detwinned CaFeAsF for which this kind of electron
phonon coupling effect should be even stronger since the Fe-As
phonon mode is closer to the electronic singularity.

**IV. CONCLUSION**

To summarize, the optical conductivity of CaFeAsF single crystal has been measured as a function of temperature and over a broad frequency range. We have studied how the spectral fea-tures associated with the SDW gap develop across the structural and magnetic transitions. In the SDW state we have observed a singular absorption feature and two regions of quasilinear con-ductivity that have been interpreted in terms of the response of Dirac fermions. We also showed that these features disappear very rapidly as a function of electron and hole doping in the BaFe2As2 system. In CaFeAsF we have furthermore found that the infrared-active Fe-As phonon mode shows signatures of a strong coupling with the Dirac fermions that appear in the SDW state. The strength of this electron phonon coupling can be material dependent, since it strongly depends on the relative position of the electronic singularity and the phonon mode, and can also be strongly anisotropic with respect to the polarization of the light, i.e., whether it is parallel or perpendicular to the line that connects the pair of Dirac cones.

**ACKNOWLEDGMENTS**

Work at HPSTAR was supported by NSAF, Grant No. U1530402. Work at the University of Fribourg was sup-ported by the Schweizer Nationalfonds (SNF) by Grant No. 200020-172611. G.M. is supported by the Youth Innovation Promotion Association of the Chinese Academy of Sciences (No. 2015187).

[1] Y. Kamihara, T. Watanabe, M. Hirano, and H. Hosono,J. Am.
**Chem. Soc. 130**,3296(2008).

[2] J. Paglione and R. L. Greene,**Nat. Phys. 6**,645(2010).
[3] I. I. Mazin, D. J. Singh, M. D. Johannes, and M. H. Du,Phys.

**Rev. Lett. 101**,057003(2008).

[4] K. Kuroki, S. Onari, R. Arita, H. Usui, Y. Tanaka, H. Kontani,
and H. Aoki,**Phys. Rev. Lett. 101**,087004(2008).

[5] H. Ding, P. Richard, K. Nakayama, K. Sugawara, T. Arakane,
*Y. Sekiba, A. Takayama, S. Souma, T. Sato, T. Takahashi et al.,*
**Europhys. Lett. 83**,47001(2008).

[6] J. G. Analytis, R. D. McDonald, J.-H. Chu, S. C. Riggs, A. F.
Bangura, C. Kucharczyk, M. Johannes, and I. R. Fisher,Phys.
**Rev. B 80**,064507(2009).

[7] Y. Ran, F. Wang, H. Zhai, A. Vishwanath, and D.-H. Lee,Phys.
**Rev. B 79**,014505(2009).

[8] Z. P. Yin, K. Haule, and G. Kotliar, **Nat. Phys. 7**, 294
(2011).

[9] P. Richard, K. Nakayama, T. Sato, M. Neupane, Y.-M. Xu, J. H.
*Bowen, G. F. Chen, J. L. Luo, N. L. Wang, X. Dai et al.,*Phys.
**Rev. Lett. 104**,137001(2010).

[10] N. Harrison and S. E. Sebastian, **Phys. Rev. B 80**, 224512
(2009).

[11] T. Morinari, E. Kaneshita, and T. Tohyama,**Phys. Rev. Lett. 105**,
037203(2010).

[12] K. K. Huynh, Y. Tanabe, and K. Tanigaki,**Phys. Rev. Lett. 106**,
217004(2011).

[13] Z.-G. Chen, L. Wang, Y. Song, X. Lu, H. Luo, C. Zhang, P. Dai,
Z. Yin, K. Haule, and G. Kotliar,**Phys. Rev. Lett. 119**,096401
(2017).

[14] A. Damascelli, Z. Hussain, and Z.-X. Shen,**Rev. Mod. Phys. 75**,
473(2003).

[15] S. Y. Zhou, G.-H. Gweon, J. Graf, A. V. Fedorov, C. D. Spataru,
R. D. Diehl, Y. Kopelevich, D.-H. Lee, S. G. Louie, and A.
Lanzara,**Nat. Phys. 2**,595(2006).

[16] M. Z. Hasan and C. L. Kane,**Rev. Mod. Phys. 82**,3045(2010).
[17] X.-L. Qi and S.-C. Zhang,**Rev. Mod. Phys. 83**,1057(2011).
[18] G. Xu, H. Weng, Z. Wang, X. Dai, and Z. Fang,Phys. Rev. Lett.

**107**,186806(2011).

[19] X. Wan, A. M. Turner, A. Vishwanath, and S. Y. Savrasov,Phys.
**Rev. B 83**,205101(2011).

[20] Y. Xiao, Y. Su, R. Mittal, T. Chatterji, T. Hansen, C. M. N. Kumar, S. Matsuishi, H. Hosono, and T. Brueckel,Phys. Rev. B

**79**,060504(2009).

[21] Y. Ma, H. Zhang, B. Gao, K. Hu, Q. Ji, G. Mu, F. Huang, and X.
Xie,**Supercond. Sci. Technol. 28**,085008(2015).

[22] M. Rotter, M. Tegel, D. Johrendt, I. Schellenberg, W. Hermes,
and R. Pöttgen,**Phys. Rev. B 78**,020503(2008).

[23] S. Matsuishi, Y. Inoue, T. Nomura, H. Yanagi, M. Hirano, and
H. Hosono,**J. Am. Chem. Soc. 130**,14428(2008).

[24] P. Cheng, B. Shen, G. Mu, X. Zhu, F. Han, B. Zeng, and H.-H.
Wen,**Europhys. Lett. 85**,67003(2009).

[25] W. Z. Hu, J. Dong, G. Li, Z. Li, P. Zheng, G. F. Chen, J. L. Luo,
and N. L. Wang,**Phys. Rev. Lett. 101**,257005(2008).
[26] A. Charnukha, D. Pröpper, T. I. Larkin, D. L. Sun, Z. W. Li,

C. T. Lin, T. Wolf, B. Keimer, and A. V. Boris,**Phys. Rev. B 88**,
184511(2013).

[27] Y. M. Dai, A. Akrap, S. L. Bud’ko, P. C. Canfield, and C. C.
Homes,**Phys. Rev. B 94**,195142(2016).

[28] A. Akrap, J. J. Tu, L. J. Li, G. H. Cao, Z. A. Xu, and C. C. Homes,
**Phys. Rev. B 80**,180502(2009).

[29] M. Nakajima, T. Liang, S. Ishida, Y. Tomioka, K. Kihou, C. H.
*Lee, A. Iyo, H. Eisaki, T. Kakeshita, T. Ito et al.,*Proc. Natl.
**Acad. Sci. 108**,12238(2011).

[30] A. A. Schafgans, B. C. Pursley, A. D. LaForge, A. S. Sefat, D.
Mandrus, and D. N. Basov,**Phys. Rev. B 84**,052501(2011).
[31] B. Xu, Y. M. Dai, B. Shen, H. Xiao, Z. R. Ye, A. Forget, D.

*Colson, D. L. Feng, H. H. Wen, C. C. Homes et al.,*Phys. Rev.
**B 91**,104510(2015).

[32] B. Xu, Y. M. Dai, H. Xiao, B. Shen, Z. R. Ye, A. Forget, D.
*Colson, D. L. Feng, H. H. Wen, X. G. Qiu et al.,*Phys. Rev. B

**94**,085147(2016).

[33] B. P. P. Mallett, C. N. Wang, P. Marsik, E. Sheveleva, M.
Yazdi-Rizi, J. L. Tallon, P. Adelmann, T. Wolf, and C. Bernhard,Phys.
**Rev. B 95**,054512(2017).

[34] B. Shen, H. Yang, Z.-S. Wang, F. Han, B. Zeng, L. Shan, C. Ren,
and H.-H. Wen,**Phys. Rev. B 84**,184512(2011).

[35] F. Rullier-Albenque, D. Colson, A. Forget, and H. Alloul,Phys.
**Rev. Lett. 103**,057001(2009).

[36] C. C. Homes, M. Reedyk, D. A. Cradles, and T. Timusk,Appl.
**Opt. 32**,2976(1993).

*[37] M. Dressel and G. Grüner, Electrodynamics of Solids*
(Cambridge University Press, Cambridge, 2002).

[38] Z. G. Chen, R. H. Yuan, T. Dong, and N. L. Wang,Phys. Rev. B

**81**,100502(2010).

[39] T. Dong, Z. G. Chen, R. H. Yuan, B. F. Hu, B. Cheng, and N. L.
Wang,**Phys. Rev. B 82**,054522(2010).

[40] F. Ma, Z.-Y. Lu, and T. Xiang, **Phys. Rev. B 78**, 224517
(2008).

[41] C. Fang, H. Yao, W.-F. Tsai, J. P. Hu, and S. A. Kivelson,Phys.
**Rev. B 77**,224509(2008).

[42] C. Xu, M. Müller, and S. Sachdev,**Phys. Rev. B 78**,020501
(2008).

[43] P. Hosur, S. A. Parameswaran, and A. Vishwanath,Phys. Rev.
**Lett. 108**,046602(2012).

[44] T. Timusk, J. P. Carbotte, C. C. Homes, D. N. Basov, and S. G.
Sharapov,**Phys. Rev. B 87**,235121(2013).

[45] C. J. Tabert and J. P. Carbotte, **Phys. Rev. B 93**, 085442
(2016).

[46] B. Xu, Y. M. Dai, L. X. Zhao, K. Wang, R. Yang, W. Zhang,
*J. Y. Liu, H. Xiao, G. F. Chen, A. J. Taylor et al.,*Phys. Rev. B

**93**,121110(2016).

[47] S. I. Kimura, H. Yokoyama, H. Watanabe, J. Sichelschmidt,
V. Süß, M. Schmidt, and C. Felser,**Phys. Rev. B 96**,075119
(2017).

[48] T. Terashima, H. T. Hirose, D. Graf, Y. Ma, G. Mu, T. Hu, K.
Suzuki, S. Uji, and H. Ikeda, **Physical Review X 8**, 011014
(2018).

[49] K. Sugimoto, E. Kaneshita, and T. Tohyama,J. Phys. Soc. Jpn.

**80**,033706(2011).

[50] K. F. Mak, M. Y. Sfeir, Y. Wu, C. H. Lui, J. A. Misewich, and
T. F. Heinz,**Phys. Rev. Lett. 101**,196405(2008).

[51] A. B. Kuzmenko, E. van Heumen, F. Carbone, and D. van der
Marel,**Phys. Rev. Lett. 100**,117401(2008).

[52] U. Fano,**Phys. Rev. 124**,1866(1961).

[53] S. Sim, N. Koirala, M. Brahlek, J. H. Sung, J. Park, S. Cha, M.-H.
Jo, S. Oh, and H. Choi,**Phys. Rev. B 91**,235438(2015).
[54] A. D. LaForge, A. Frenzel, B. C. Pursley, T. Lin, X. Liu, J. Shi,

and D. N. Basov,**Phys. Rev. B 81**,125120(2010).

[55] B. Xu, Y. M. Dai, L. X. Zhao, K. Wang, R. Yang, W. Zhang, J. Y.
*Liu, H. Xiao, G. F. Chen, S. A. Trugman et al.,*Nat. Commun.

**8**,14933(2017).